Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.


 Lucas Short
 1 years ago
 Views:
Transcription
1 49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates. C. B. York * University of Glasgow, Glasgow, Scotland, G12 8QQ Stacking sequence listings are presented for fully uncoupled Extensionally Isotropic (EILs), Fully Isotropic (FILs) and QuasiHomogeneous Orthotropic (QHOLs) angleply Laminates, with up to 21 plies. All are subsets of a definitive list of Fully Orthotropic Laminates (FOLs), containing generally nonsymmetric stacking sequences that are characterized in terms of angle and crossply subsequence symmetries. Dimensionless parameters are given for each stacking sequence, from which the ABD matrix is readily derived. Expressions relating these dimensionless parameters to the wellknown lamination parameters are also given, together with graphical representations of the feasible domains for π/3 and π/4 EILs and angleply QHOLs containing two and three ply orientations. The feasible domain for π/3 FILs is represented graphically by a single point, whereas the domain for angleply QHOLs containing four ply orientations is represented by a single stacking sequence. Nomenclature A,A ij = extensional (membrane) stiffness matrix and its elements (i,j = 1, 2, 6) B,B ij = bendingextensioncoupling stiffness matrix and its elements (i,j = 1, 2, 6) D,D ij = bending (flexural) stiffness matrix and its elements (i,j = 1, 2, 6) H = laminate thickness (= n t) n = number of plies in laminate stacking sequence N x,n y = inplane axial load per unit length. N xy = inplane shear flow. M x,m y = bending moments per unit length about principal axes. M xy = twist moment per unit length. Q ij = reduced stiffness (i,j = 1, 2, 6) Q ij = transformed reduced stiffness (i,j = 1, 2, 6) t = ply thickness x,y,z = principal axes ε x,ε y = inplane axial strains. γ xy = inplane shear strain. κ x,κ y = curvatures about principal axes. κ xy = twist curvature. ξ 1,ξ 2 = lamination parameters for extensional stiffness (ξ 1 = ξ A 1,ξ 2 = ξ A 2 ) ξ 9,ξ 10 = lamination parameters for bending stiffness (ξ 9 = ξ D 1, ξ 10 = ξ D 2 ) ζ,ζ ±,ζ,ζ = bending stiffness parameter for laminate, and angleply and crossply subsequences +,,± = angle plies, used in stacking sequence definition, = crossplies, used in stacking sequence definition Matrix subscripts 0 = All elements zero F = All elements finite I = Isotropic form, see Eqs. (5) (7) S = Specially orthotropic form, see Eqs. (3)  (4) * Senior Lecturer, Department of Aerospace Engineering, James Watt Building. 1 Copyright 2008 by C. B. York. Published by the, Inc., with permission.
2 Keywords Stacking Sequences; Fully Uncoupled Laminates; Extensionally (or Membrane or Quasi) Isotropic Laminates; Fully Isotropic Laminates; Bending Stiffness Parameters; Lamination Parameters; Feasible Domains. I. Introduction omposite laminate materials are typically characterized in terms of their response to mechanical (and/or thermal) loading, which is generally associated with a description of the coupling behavior, unique to this type C of material, i.e. coupling between inplane (i.e. extension or membrane) and outofplane (i.e. bending or flexure) responses when B ij 0 in Eq. (1), coupling between inplane shear and extension when A 16 = A 26 0, and coupling between outofplane bending and twisting when D 16 = D N N N x y xy A11 A12 A16 ε x = A22 A26 ε y + Sym. A66 τ xy B11 Sym. B B B B B κ x κ y κ xy M M M x y xy B11 B12 B16 ε x D11 D12 D16 κ x = B22 B26 ε y + D22 D26 κ y (1) Sym. B66 τ xy Sym. D 66 κ xy Whilst Eq. (1) describes the wellknown ABD relation from classical laminate plate theory, it is more often expressed using compact notation: N M A B ε = (2) B D κ The coupling behavior, which is dependent on the form of the elements in each of the extensional (A), coupling (B) and bending (D) stiffness matrices is now described by an extended subscript notation, defined previously by the Engineering Sciences Data Unit, or ESDU 1 and subsequently augmented for the purposes of this article. Hence, balanced and symmetric stacking sequences, which generally possess bending anisotropy, give rise to coupling between outofplane bending and twisting and are referred to by the designation A S B 0 D F, signifying that the elements of the extensional stiffness matrix (A) are specially orthotropic in nature, i.e. uncoupled, since A 16 = A 26 = 0, (3) the bendingextension coupling matrix (B) is null, whilst all elements of the bending stiffness matrix (D) are finite, i.e. D ij 0. Laminates possessing extensional anisotropy give rise to coupling between inplane shear and extension only and, by the same rationale, are referred to by the designation A F B 0 D S, signifying that all elements of the extensional stiffness matrix (A) are finite, i.e. A ij 0, the bendingextension coupling matrix (B) is null, and the elements of the bending stiffness matrix (D) are specially orthotropic in nature, i.e. uncoupled, since D 16 = D 26 = 0 (4) The A F B 0 D S designation is not listed as part of the ten laminate classifications described in the ESDU data item 1, but is however the subject of a recent article 2, identifying the definite list of A F B 0 D S stacking sequences with up to 21 plies, thus complementing a new definitive list 3 of Fully Orthotropic Laminates or FOLs. Note that the term for FOLs is synonymous with specially orthotropic laminates, which possess none of the coupling characteristics described above and are represented by the designation A S B 0 D S. 2
3 This article presents the characterization of uncoupled Extensionally Isotropic Laminates or EILs, with the designation A I B 0 D S and Fully Isotropic Laminates or FILs, with the designation A I B 0 D I. These laminates represent subsets of FOLs and are therefore contained within the definitive list 3, since in addition to the specially orthotropic form of each matrix, see Eq. (3), elements simplify further in EILs and the designation A S is replaced with A I to indicate that: and A 11 = A 22 (5) A 66 = (A 11 A 12 )/2 (6) and further still in FILs, in which the designation D S is replaced with D I to indicate that: D ij = A ij H 2 /12, (7) where H is the laminate thickness, corresponding to the total number of plies, n, of thickness t. QuasiHomogeneous Orthotropic Laminates, or QHOLs, similar to the QuasiHomogeneous Anisotropic Laminates, or QHALs, described and patented by Wu and Avery 5, satisfy Eq. (7) but not Eqs. (5) and/or (6). QHOLs (QHALs) offer matching orthotropy (anisotropy) in both extensional and bending stiffness. Note that QHOLs are developed herein for general ply angle ±θ, but the same stacking sequences produce QHALs when +θ θ. Fully orthotropic laminates, from which all stacking sequences presented in this article are derived, minimize distortion during manufacturing and maximize compression buckling strength 6, particularly in comparison to balanced and symmetric laminates, which are commonly adopted in aircraft and spacecraft construction, despite the fact that such laminates generally possess bending anisotropy. Valot and Vannucci provide recent examples of laminate stacking sequences for FOLs with antisymmetric sequences 7, following a previous article 8 on FILs. These two articles are part of, and provide reference to, a growing number of related articles by a community of coworkers addressing the development of laminate stacking sequences exhibiting a range of physical characteristics, all of which refer back to an original article by Caprino and CrivelliVisconti 9, identifying the specially orthotropic angleply laminate with eight plies. Much of this related work has been focused on laminate stacking sequences for QuasiIsotropic or Extensionally Isotropic Laminates (EILs), Fully Isotropic Laminates (FILs), and laminates with material homogeneity. However, with the exception of FILs, these material characterizations generally provide little or no distinction between laminates with or laminates without coupling behavior. For instance, the quasihomogenous laminate, which is defined as possessing the same elastic propertied in both flexural and membrane actions, but with no coupling between these two actions, may be designated as either A F B 0 D F or A S B 0 D S, and extensionally isotropic laminate may be designated as either A I B 0 D F or A I B 0 D S. Such sequences have been obtained through an inverse polar (or Mohr s circle) representation method developed by Verchery and coworkers, which is acknowledged 10 to be similar to the method presented previously by Tsai and Pagano 11. By contrast, original work by Bartholomew 12,13, which forms the basis of the Engineering Sciences Data Unit (ESDU) publication 14 for the so called definitive list of fully orthotropic angleply laminates with designation A S B 0 D S, precedes the findings of Caprino and CrivelliVisconti 9, but appears to have been completely overlooked in the literature described above. This published list of stacking sequences contains 75 symmetric sequences for laminates with up to 21 plies, 653 antisymmetric sequences for laminates with up to 20 plies and 49 additional nonsymmetric (asymmetric) sequences, which were derived by combining the symmetric and antisymmetric sequences. Further inspection reveals that there are no angleply laminates possessing specially orthotropic properties with fewer than 7 plies. Indeed, there is only one generic 7layer angleply antisymmetric stacking sequence. This number increases to 233 generic antisymmetric sequences with 20 ply layers. There are no symmetric stacking sequences with less than 12 layers, and only 25 combinations with 20 layers. These twentyfive generic stacking sequences possess balanced and symmetric combinations of angle plies, together with cross plies, which may be 0 and/or 90, symmetrically disposed about the laminate midplane; all possess angleply layers on the outer surfaces of the laminate. The term generic is used here to describe the form of the stacking sequences adopted, defined by three parameters: +, and, relating to positive and negative angle plies with general orientation, θ, and cross ply, respectively. The derivation 12,13 adopted in the ESDU data item 14, made the explicit assumption that cross plies, as well as angle plies, are symmetrically disposed about the laminate midplane, i.e. the mixing of 0 and 90 plies is 3
4 permitted only in one half of the laminate, which is then reflected symmetrically about the laminate midplane. This rule applies to both symmetric and antisymmetric angleply stacking sequences. For this reason, cross plies are legitimately represented by the single parameter. The relatively small number of fully orthotropic sequences for thin laminates clearly leaves limited scope for composite tailoring, particularly where ply terminations are necessary and fully orthotropic characteristics are a design requirement. This was the key motivation leading to the redevelopment of the definitive list 3 for specially orthotropic angleply laminates with up to 21 plies, which is presented in a related article in abridged form 4. In the derivation of this list for (but not restricted to) standard angleply configurations, i.e. ±45, 0 and 90, the general rule of symmetry is relaxed. Crossplies, as well as angleplies, are therefore no longer constrained to be symmetric about the laminate midplane, leading to an increase in the number of possible solutions. For 16ply laminates, there are approximately one million possible stacking sequence combinations, of which 368 comply with the requirements of special orthotropy, increasing to approximately 1 billion combinations for 21 plies, giving rise to a hundredfold increase in the number of fully orthotropic laminates. Because of the substantial number of sequences identified in the definitive list, it is beneficial, for design purposes, to express the stiffness properties in terms of lamination parameters, which can be conveniently presented in graphical form, as originally conceived by Fukunaga and Vanderplaats 15 for the purposes of optimum design: the flexural stiffness terms are now fully defined by two linear design variables. Optimized lamination parameters may then be matched against a corresponding set of stacking sequences for a given laminate thickness H (= n t). These graphical representations of feasible domains are readily extended to other laminate classifications: EILs with π/3 ply separation are reduced to a single line representation, whilst π/3 FILs are represented by a single point. II. Stacking sequence derivation In the derivation of the stacking sequences that follow, the general rule of symmetry is relaxed. Cross plies, as well as angle plies, are therefore no longer constrained to be symmetric about the laminate midplane. Consequently, the mixing of 0 and 90 plies needs special attention to avoid violation of the rules for special orthotropy, see Eqs. (3)  (4). There are many nonsymmetric forms contained in the definitive list of fully orthotropic laminates for standard angleply configurations, e.g. ±45, 0 and 90, being both extraordinary in appearance and seemingly infeasible in terms of the uncoupled behavior that the laminates possess. The great majority of sequences are nonsymmetric and many of these are without any subsequence patterns, which is contrary to the assumptions on which many previous studies have been based. Arrangement and form of stacking sequence data For compatibility with the previously published data, similar symbols have been adopted for defining all stacking sequences that follow. Additional symbols and parameters are necessarily included to differentiate between cross plies (0 and 90 ), given that symmetry about the laminate midplane is no longer assumed. The resulting sequences are characterized by subsequence symmetries using a double prefix notation, the first character of which relates to the form of the angleply subsequence and the second character to the crossply subsequence. The double prefix contains combinations of the following characters: A to indicate Antisymmetric form; N for Nonsymmetric; and S for Symmetric. Additionally, for crossply subsequence only, C is used to indicate Crosssymmetric form. To avoid the trivial solution of a stacking sequence with cross plies only, all sequences have an angleply (+) on one outer surface of the laminate. As a result, the other outer surface may have an angleply of equal (+) or opposite ( ) orientation or a cross ply ( ), which may be either 0 or 90. A subscript notation, using these three symbols, is employed to deferential between similar forms of sequence. The form (and number) of FOL stacking sequences contained in the definitive list 3 for up to 21 plies can be summarized as: AC (210), AN (14,532), AS (21,906), SC (12), SN (192), SS (1,029), + NS + (220), + NS (296), + NN + (5,498), + NN (15,188) and + NN = + NN (10,041). From these sequence listings, the form (and number) of the subset for fully uncoupled EIL stacking sequences with π/3 isotropy can be summarized as: AS (173), SS (10), + NN + (106), + NN (208) and + NN = + NN (238), whilst the form (and number) of EIL stacking sequences with π/4 isotropy can be summarized as: AC (12), AS (72), SC (2), SS (6) and + NN = + NN (6). Angleply QHOLs containing a single crossply orientation, i.e. +, and only, can be summarized as: AS (28), SS (4), + NS + (4), + NN + (8), + NN (4) and + NN = + NN (16). 4
5 Development of parameters As adopted in the published ESDU listings 14, the new sequences are ordered in terms of ascending numbers of plies, n, or ζ (= n 3 ), which are in turn ordered by ascending value of the bending stiffness parameter for the angle plies (ζ ± ) and finally by one of the two crossply subsequences (ζ ) within the laminate. Hence, the numbering of sequences for each subsymmetric form, described in the previous section, may be readily extended for higher numbers of plies. All sequences presented in the current article retain their original FOL reference number. The calculation of the bending stiffness parameter, ζ ±, is readily demonstrated for the 9ply fully uncoupled π/3 EIL, designated A382 in the ESDU listings 14 and AS 7 in the definitive list 3, with stacking sequence [±/ / / /+/ /±] T, where the bending stiffness terms, n D ij = Q ij (z k 3 z k1 3 )/3 (8) k = 1 may be written in sequence order for the 9 individual plies, where z, representing the distance from the laminate midplane, is expressed here in terms of the uniform ply thickness t: D ij = {Q ij+ ((7t/2) 3 (9t/2) 3 ) + Q ij ((5t/2) 3 (7t/2) 3 ) + Q ij ( (3t/2) 3 (5t/2) 3 ) + Q ij ((t/2) 3 (3t/2) 3 ) + Q ij ((t/2) 3 (t/2) 3 ) + Q ij+ ((3t/2) 3 (t/2) 3 ) + Q ij ((5t/2) 3 (3t/2) 3 ) + Q ij+ ((7t/2) 3 (5t/2) 3 ) + Q ij ((9t/2) 3 (7t/2) 3 )}/3 (9) where subscripts i, j = 1, 2, 6. The bending stiffness contribution from the angle plies is therefore: and for crossplies: These bending stiffness terms are written in alternative form in Ref. 14 as: and D ij± = 157.5t 3 /3 Q ij± (10) D ij = 24.75t 3 /3 Q ij (11) D ij± = ζ ± t 3 /12 Q ij± (12) D ij = ζ t 3 /12 Q ij (13) respectively, since the number of plies (n = 9) is now related directly to the bending stiffness terms by the expression: ζ ± + ζ = ζ = n 3 (14) where ζ ± = 630 and ζ = n 3 = 729, hence ζ = 99. The stiffness parameters are hereby extended to incorporate both crossplies (ζ and ζ ), including percentage values to indicate the relative proportion (n ± /n, n /n and n /n) and relative contribution to bending stiffness (ζ ± /ζ, ζ /ζ and ζ /ζ) of each ply subsequences within the laminate, i.e. a subsequence containing either ±, or plies. These relationships also help to identify other laminate properties, which are subsets of FOLs. For instance, a QuasiHomogeneous Orthotropic Laminate, or QHOL, has n ± /n = ζ ± /ζ, n /n = ζ /ζ and n /n = ζ /ζ; a π/3 (π/4) 5
6 Extensionally Isotropic Laminate, or EIL, has n ± /n = 2n /n (or = n /n = n /n) and; a π/3 Fully Isotropic Laminate, or FIL, has n ± /n = 2n /n = ζ ± /ζ = 2ζ /ζ. The set of FOLs with up to 21 plies contains no π/4 FILs. Validation The definitive list of FOL stacking sequences, from which the subsets of EILs FILs and QHOLs are derived, have been validated against the published ESDU listing 14, containing symmetric (SS) and antisymmetric (AS) laminates, together with a limited number of nonsymmetric sequences. The laminates detailed in Refs 7, 8, 10 and 16, which have been algorithmically filtered to provide mathematically and mechanically unique stacking sequences, provide further validation. Applying this filtering to the 18 FILs, with π/3 isotropy, identified as a subset of FOLs, which are of the form (and number) + NN + (2), + NN (8) and + NN (8), reveals that: only 1 of the 2 + NN + sequences is unique when the order is reversed, see Fig. 1; only 4 from the 8 + NN sequences are unique when the order is reversed and + and plies are interchanged, see Fig. 2 and; + NN sequences are identical to + NN sequences with and plies interchanged, see Fig. 3, leaving the 5 mathematically and mechanically unique sequences identified by Vannucci and Verchery 8, i.e.: (NN 1071) (NN 1073) (NN 1074) (NN 1075) (NN 1077) [±/ / 3 /+ 2 / /m/±/ 2 / 2 /+] T [+/ / 2 / /+/ /m/±/ /m/ 2 /±] T [+/ / / /m 2 / / / /+/±/ 2 /±] T [+/ 2 / 2 /±/m/+/ 3 /±/ /±] T [+/ / / /m 2 / /m/ 2 /m/+/ / ] T in which +/ / are presented as +60/ 60/0, respectively, in the feasible domains of lamination parameters that follow, but may indeed be any combination of ply angles with π/3 separation; the designations in parentheses correspond to the FOL sequences of Ref. 3. However, the notion of mathematically and mechanically unique stacking sequences is believed to be of limited practical significance, particularly in view of the identical stress distributions of sequences #1 and #4 of Ref. 8, illustrated in Figs 3(g) and 3(e), respectively. This situation arises because the crossply subsequences are identical in these two laminates and, for the particular load combination used, the stress distribution is insensitive to the angleply subsequence. Similarly, laminates NN 1073, 1075, 1081 and 1082, of Figs 2(a), 2(c), 3(c) and 3(a) respectively, have identical stress distributions for the same load combination when the material axis is rotated through 60, i.e. +/ / now represent 0/60/ 60, because the crossply subsequences are identical in all four laminates (a) NN 1071: (b) NN 1071 NN 1072 #5: [±/ / 3 /+ 2 / /m/±/ 2 / 2 /+] T [+/ 2 / 2 /m/±/ /+ 2 / 3 / /m] T Figure 1 Through the thickness stress distribution for fully isotropic, unrestrained laminate (a) NN 1071, and (b) NN 1072 when stacking sequence is reversed, giving rise to sequence #5 of Ref
7 (a) NN 1073: [+/ / 2 / /+/ /m/±/ /m/ 2 /±] T (b) NN 1074: [+/ / / /m 2 / / / /+/±/ 2 /±] T (c) NN 1075: [+/ 2 / 2 /±/m/+/ 3 /±/ /±] T (d) NN 1077: [+/ / / /m 2 / /m/ 2 /m/+/ / ] T (e) NN 1073 NN 1076 [+/ / 2 / /+/ /m/±/ /m/ 2 /±] T (f) NN 1074 NN 1078: [±/ 2 /±/ / /+/ /m 2 / /+/ / ] T (g) NN 1075 NN 1080: [±/ /±/ 3 / 2 /+ 2 /m/+/ 2 / ] T (h) NN 1077 NN 1079 #2: [+/ / /m/ 2 /m/ /m 2 / /+/ / ] T Figure 2 Through the thickness stress distribution for fully isotropic, unrestrained laminates (a) (d) NN 1071 NN 1075 and NN 1077, subject to combined inplane load N x and bending moment M x, and (e) (h) NN 1076, NN 1078 NN 1080 when stacking sequence is reversed and + and plies interchanged; (h) NN 1079 represents sequence #2 of Ref. 8. 7
8 (a) NN 1073 NN 1082: [±/ 2 / /±/ /+ 2 / / / /±/m/ ] T (b) NN 1074 NN 1083: [±/ / / /+/ /±/ /m/+/ / /m/ ] T (c) NN 1075 NN 1081: [±/ / 2 /+/ 2 /+ 2 / 3 /+/ /m/ ] T (d) NN 1077 NN 1084: [±/ / / /+/ /±/ /±/ / /+/±/ ] T (e) NN 1076 NN 1085 #4 [±/ 2 /m/ /±/m/ / / /+ 2 / / ] T (f) NN 1078 NN 1087 #3: [+/ / /m/ 2 /m/ / /+/ /± 2 / ] T (g) NN 1080 NN 1088 #1: [+/ /m/ / 3 / 2 /+ 2 / /+ 2 / 2 / ] T (h) NN 1079 NN 1086: [±/ 2 /±/ / /±/ /+/ /± 2 / ] T Figure 3 Through the thickness stress distribution for fully isotropic, unrestrained laminates (a) (d) NN 1073 NN 1075 and NN 1077, subject to combined inplane load N x and bending moment M x, and (e) (h) NN 1076, NN 1078 NN 1080, resulting from those of Fig. 2 when and plies interchanged, respectively; (g), (f) and (e) giving rise to sequences #1, #3 and #4 of Ref. 8, respectively. Note the identical stress distribution of (e) and (g). 8
9 Figures 1 3 represent the through the thickness stress distributions for unrestrained fully isotropic laminated plates subject to combined inplane load N x (= 4.2 N/mm) and bending moment M x (= 10.0 N.mm/mm). Individual stress distribution profiles arising from the application of N x and M x (dashed lines) are illustrated together with the combined stress distribution profile (solid lines). Material properties and constant ply thickness, t, used in the calculation of these stress distributions, are given in the example calculations that follow. Wu and Avery 5 obtained FILs by varying, or shuffling, the stacking sequences of fully uncoupled EILs in order to produce bending isotropy. Eightynine stacking sequences were presented as the symmetric halves of 36ply laminates with fully isotropic properties, deemed to be the minimum number of plies for π/3 FILs. Limited details of 54ply sequences for FILs with π/3 isotropy are also provided, together with π/4, π/5 and π/6 isotropy for 48, 50 and 72ply sequences, respectively. The symmetry assumption, on which this work is based, precluded the possibility that the listings would contain nonsymmetric 18ply FILs. However, inspection of this list reveals that nine of these stacking sequences represent 18ply nonsymmetric FILs; the nine sequences are reproduced in Table 1 with the original reference numbers and formatting. Table 1 Stacking sequences for 18ply nonsymmetric FILs, representing the symmetric halves of 36ply FILs (after Ref. 5) Ref. θ 1 θ 2 θ Each ply number, 1 through 18, appears under the appropriate plyangle heading, θ 1, θ 2 or θ 3 in row 1 of Table 1. Sequences 57, 65, 66, 70 and 78, correspond to the 5 mechanically and mathematically distinct sequences derived independently by Vannucci and Verchery 8 some ten years later, whilst sequence 69 is sequence 65 with the order reversed and with θ 3, θ 2 and θ 1 in row 1. Similarly, sequences 73, 76 and 77 are, respectively, 66, 57 and 70 with the order reversed and with θ 2, θ 3 and θ 1 in row 1. Sequence AC 127, which is discussed in detail in section V, has special significance: It is a QHOL and validates the unique angleply laminate containing four ply orientations, i.e. +,, and, alluded to in Ref. 16 for a 20 ply laminate satisfying Eq. (7), and Eq. (5) when ply orientations satisfy the π/4 condition, but not Eq. (6). Note that AC 127 and AC 128 are identical when crossplies are interchanged, with. All other QHOLs with up to 21 plies contain either two or three ply orientations, i.e. +, or +, and, respectively. III. Stacking sequence listings The following Tables provide summaries of the numbers of fully uncoupled EIL and QHOL stacking sequences with up to 21 plies together with crossreferences to the Tables of the full sequence listings and nondimensional parameters, given in the appendix. Note that percentage values to indicate the relative proportion (n ± /n, n /n and n /n) and relative contribution to bending stiffness (ζ ± /ζ, ζ /ζ and ζ /ζ) of each ply subsequences within the laminate have been omitted for reasons of compactness, together with other parameters that are common within a given table. These missing parameters are readily calculated from the expressions provided within the table captions. 9
10 Table 2  Number of fully uncoupled π/3 EILs [π/4 EILs] for 7 through 21ply laminates, corresponding to prefix designations for Antisymmetric (A), Crosssymmetric (C), Nonsymmetric (N) and Symmetric (S) ply subsequences, listed in abridged form in Tables 7 and 8. Subscripts arranged before and after the prefix designations denote angle (+, ) and cross plies ( ), and correspond to the orientations of the top and bottom plies of the laminate respectively. Number of plies, n Prefix: Table: AC [2] /[8(a)] AS [2] (a)/[8(b)] SC [2] /[8(c)] +NN (b)/ +NN (c)/ +NN [6] (d)/[8(d)] SS [6] /[8(e)] Table 3  Number of QHOLs containing no crossply orientations for 7 through 21ply laminates, corresponding to prefix designations for Antisymmetric (A), Nonsymmetric (N) and Symmetric (S) ply subsequences, listed in Table 9. Subscripts arranged before and after the prefix designations denote angle (+, ) plies and correspond to the orientations of the top and bottom plies of the laminate respectively. Prefix: Number of plies, n Table: AS (a) +NS (b) +NS 8 9(c) SS 1 9(d) Table 4  Number of QHOLs containing one [both] crossply orientation[s] for 7 through 21ply laminates, corresponding to prefix designations for Antisymmetric (A), Crosssymmetric (C), Nonsymmetric (N) and Symmetric (S) ply subsequences, listed in Table 10. Subscripts arranged before and after the prefix designations denote angle (+, ) and cross plies ( ), and correspond to the orientations of the top and bottom plies of the laminate respectively. Prefix: Number of plies, n Table: AC [2]  AS (a) +NS (b) +NN (c) +NN 4 10(d) +NN (e) SS 4 10(f) 10
11 IV. Calculation of membrane and bending stiffness terms The calculation procedure for the elements (A ij and D ij ) of the extensional (A) and bending (D) stiffness matrices, using the dimensionless parameters provided in Tables 710, are as follows: A ij = {n ± /2 Q ij+ + n ± /2 Q ij + n Q ij + n Q ij } t (15) D ij = {ζ ± /2 Q ij+ + ζ ± /2 Q ij + ζ Q ij + ζ Q ij } t 3 /12 (16) The form of Eqs. (15) and (16) was chosen because they are readily modified to account for laminates with extensional and bending anisotropy by replacing n ± /2 Q ij+ with n ± (n + /n ± )Q ij+ and n ± /2 Q ij with n ± (1 n + /n ± )Q ij, and ζ ± /2 Q ij+ with ζ ± (ζ + /ζ ± ) Q ij+ and ζ ± /2 Q ij with ζ ± (1 ζ + /ζ ± ) Q ij. The use of these modified equation requires the calculation of an additional stiffness parameter, n + and ζ +, relating to the extensional and bending stiffness contribution of positive (θ) angle plies, respectively. The transformed reduced stiffness terms in Eqs. (15) and (16) are given by: and the reduced stiffness terms by: Q 11 = Q 11 cos 4 θ + 2(Q Q 66 )cos 2 θsin 2 θ + Q 22 sin 4 θ Q 12 = Q 21 = (Q 11 + Q 22 4Q 66 )cos 2 θsin 2 θ + Q 12 (cos 4 θ + sin 4 θ) Q 16 = Q 61 = {(Q 11 Q 12 2Q 66 )cos 2 θ + (Q 12 Q Q 66 )sin 2 θ}cosθsinθ Q 22 = Q 11 sin 4 θ + 2(Q Q 66 )cos 2 θsin 2 θ + Q 22 cos 4 θ Q 26 = Q 62 = {(Q 11 Q 12 2Q 66 )sin 2 θ + (Q 12 Q Q 66 )cos 2 θ}cosθsinθ Q 66 = (Q 11 + Q 22 2Q 12 2Q 66 )cos 2 θsin 2 θ + Q 66 (cos 4 θ + sin 4 θ) (17) Q 11 = E 1 /(1 ν 12 ν 21 ) Q 12 = ν 12 E 2 /(1 ν 12 ν 21 ) = ν 21 E 1 /(1 ν 12 ν 21 ) Q 22 = E 2 /(1 ν 12 ν 21 ) Q 66 = G 12 (18) For optimum design of angleply laminates, lamination parameters are often preferred, since these allow the stiffness terms to be expressed as linear variables. The optimized lamination parameters may then be matched against a corresponding set of stacking sequences with given laminate thickness H (= n t). In the context of the parameters presented in the current article, only four of the twelve lamination parameters are required, and these are related through the following expressions: and ξ 1 = ξ 1 A = {n ± (n + /n ± )cos(2θ + ) + n ± (1  n + /n ± )cos(2θ ) + n cos(2θ ) + n cos(2θ )}/n ξ 2 = ξ 2 A = {n ± (n + /n ± )cos(4θ + ) + n ± (1  n + /n ± )cos(4θ ) + n cos(4θ ) + n cos(4θ )}/n (19) ξ 9 = ξ 1 D = {ζ ± (ζ + /ζ ± )cos(2θ + ) + ζ ± (1  ζ + /ζ ± )cos(2θ ) + ζ cos(2θ ) + ζ cos(2θ )}/ζ ξ 10 = ξ 2 D = {ζ ± (ζ + /ζ ± )cos(4θ + ) + ζ ± (1  ζ + /ζ ± )cos(4θ ) + ζ cos(4θ ) + ζ cos(4θ )}/ζ (20) 11
12 where the extensional stiffness parameter n + = (n =) n ± /2 and bending stiffness parameters ζ + (= ζ ) = ζ ± /2 for FOLs, QHOLs, EILs and FILs, hence Eqs. (19) and (20) reduce to: and ξ 1 = {n ± cos(2θ ± ) + n cos(2θ ) + n cos(2θ )}/n ξ 2 = {n ± cos(4θ ± ) + n cos(4θ ) + n cos(4θ )}/n (21) ξ 9 = {ζ ± cos(2θ ± ) + ζ cos(2θ ) + ζ cos(2θ )}/ζ ξ 10 = {ζ ± cos(4θ ± ) + ζ cos(4θ ) + ζ cos(4θ )}/ζ (22) Elements of the extensional and bending stiffness matrices are related to the lamination parameters, respectively, by: and A 11 = {U 1 + ξ 1 U 2 + ξ 2 U 3 } H A 12 = A 21 = {ξ 2 U 3 + U 4 } H A 22 = {U 1 ξ 1 U 2 + ξ 2 U 3 } H A 66 = {ξ 2 U 3 + U 5 } H (23) D 11 = {U 1 + ξ 9 U 2 + ξ 10 U 3 } H 3 /12 D 12 = {U 4 ξ 10 U 3 } H 3 /12 D 22 = {U 1 ξ 9 U 2 + ξ 10 U 3 } H 3 /12 D 66 = {ξ 10 U 3 + U 5 } H 3 /12 (24) where the laminate invariants are given in terms of the reduced stiffnesses of Eq. (18) by: U 1 = {3Q Q Q Q 66 }/8 U 2 = {Q 11 Q 22 }/2 U 3 = {Q 11 + Q 22 2Q 12 4Q 66 }/8 U 4 = {Q 11 + Q Q 12 4Q 66 }/8 U 5 = {Q 11 + Q 22 2Q Q 66 }/8 (25) 12
13 V. Results and Discussion Figure 4(a) (d) illustrates the feasible domains of lamination parameters for all EIL and QHOL subsets from the definitive list of FOLs, in which the +/ / / of Tables 710 correspond to 45/45/0/90, respectively, or 60/ 60/0 for laminates with only one crossply orientation, e.g. π/3 EILs. All membrane (extensional) lamination parameters are bounded by the parabola ξ 2 = 2ξ with limits 1 ξ 1 1and 1 ξ 2 1; for flexural (bending) lamination parameters, ξ 9 and ξ 10 replace ξ 1 and ξ 2, respectively. Stacking sequences lying along the broken line drawn between (ξ 1, ξ 2 ) = (1, 1) and (0, 1) on Fig. 4(a), contain only 0 and ±45 plies, whereas any sequences lying along the line between (0, 1) and (1, 1) would consist of ±45 and 90 plies only. Similarly, any stacking sequences corresponding to the points (1, 1), (0, 1) or (1, 1), would contain only 90 plies, ±45 plies or 0 plies, respectively. A π/3 EIL with 2n ± = n plies, lies at the ⅓ rd point along the line defining a laminate containing only ±60 and 0 plies, i.e. (ξ 1, ξ 2 ) = (0, 0). The flexural lamination parameters corresponding to uncoupled π/3 EILs have orthotropic properties which lie along the line defined by (ξ 9, ξ 10 ) = (1, 1) and (, ) on Fig. 4(b), since the three ply orientations +/ / have been equated to 60/60/0. The flexural lamination parameters corresponding to uncoupled π/4 EILs, illustrated on Fig. 4(c), are contained within the domain defined by the three points corresponding to the 90, ±45 and 0 plies that these sequences contain, cf. Fig. 4(a). All π/3 FILs, with 2ζ ± = ζ, correspond to the point (ξ 1, ξ 2 ) = (ξ 9, ξ 10 ) = (0, 0). QHOLs correspond to any point satisfying (ξ 1, ξ 2 ) = (ξ 9, ξ 10 ) (0, 0). Degenerative QHOLs therefore result from FILs when the π/3 angle separation is relaxed, e.g. where the three ply orientations +/ / correspond to 45/45/0 rather than 60/60/0 : Such sequences are illustrated by the locus of ⅓ rd points shown by the brokenline parabola on Fig. 4(a), representing arbitrary angleply ±θ ±75 ±15 ξ ±60 ±30 ξ ± (a) Domains of membrane lamination parameters for EILs (and FILs with ξ 1 = ξ 2 = 0) and locus (brokenline parabola) for degenerative QHOLs 1.0 ξ 1 (b) Flexural lamination parameters for EILs  π/3 (973) 1.0 ξ 9 ξ ξ2, ξ ξ 9 ξ 1, ξ 9 (c) Flexural lamination parameters for EILs  π/4 (92) (d) Membrane and Flexural lamination parameters for QHOLs (82) with ±θ = 45 ( ) and ±60 ( ) Figure 4 Feasible domains of lamination parameters, in the form of Eqs. (22), for: (a) (c) EILs, including form and number of sequences represented and; (d) the subset of QHOLs from the definitive list of FOLs. 13
14 For IM7/8552 carbonfiber/epoxy material with Young s moduli E 1 = 161.0GPa and E 2 = 11.38GPa, shear modulus G 12 = 5.17GPa and Poison ratio ν 12 = 0.38, lamina thickness t = mm and stacking sequence AC 127: [+/ / 2 / / / / / / /+/ / /+/ /+/ 2 / / ] Τ, the nondimensional parameters are verified by the calculations presented in Table 5, where the first two columns provide the ply number and orientation, respectively. Subsequent columns illustrate the summations, for each ply orientation, of (z k z k1 ), (z k 2 z k1 2 )/2 and (z k 3 z k1 3 )/3, relating to the A, B and D matrices, respectively. The distance from the laminate midplane, z, is expressed in term of ply thickness t, which is set to unit value in the nondimensional expressions. Table 5 Calculation procedure for the nondimensional parameters of the ABD relation. Ply θ (z k z k1 ) A B D AΣ + A Σ A Σ AΣ BΣ + B Σ B Σ BΣ DΣ + D Σ D Σ DΣ 2 (zk z 2 k1 )/2 3 (zk z 3 k1 )/ The nondimensional parameters arising from the summations of Table 5 are: n + (= A Σ + ) = n ± /2 = 4, n = 4, n = 6 and n = 6, and ζ + (= 4 D Σ + ) = 1600, ζ = 1600, ζ = 2400 and ζ = 2400, where n 3 = 20 3 = ζ = ζ + + ζ + ζ + ζ = 8000 and ζ ± = ζ + + ζ = The B matrix summations confirm that B ij = 0 for this laminate. For fiber angles θ = ±45, 0 and 90 in place of symbols ±, and respectively, the transformed reduced stiffnesses are given in Table 6, which are readily calculated using Eqs. (17). 14
15 Table 6 Transformed reduced stiffnesses (N/mm 2 ) for IM7/8552 carbonfiber/epoxy with ply angle θ. θ Q 11 Q 12 Q 16 Q 22 Q 26 Q ,894 40,55437,791 50,89437,791 41, ,894 40,554 37,791 50,894 37,791 41, ,660 4, , , ,497 4, , ,170 and through Eqs. (15) and (16), the final stiffness matrices are derived for the laminate: A11 Sym. A A A A A ,858 52,647 0 = 202,858 0 N/mm Sym. 54,885 D11 Sym. D D D D D ,966 34,249 0 = 131,966 0 N.mm Sym. 35,705 given that: A 16 = {n + Q n Q 16 + n Q 16 + n Q 16 } t A 16 = A 26 = {4 37, , } = 0 N/mm D 16 = {ζ ± /2 Q ζ ± /2 Q 16 + ζ Q 16 + ζ Q 16 } t 3 /12 D 16 = D 26 = { , , } /12 = 0 N.mm This laminate appears to be fully isotropic, since A 11 = A 22 and D ij A ij, but calculation reveals that whilst Eqs. (5) and (7) are satisfied, Eq. (6) is not. Hence this is a Quasi Homogeneous Orthotropic angleply Laminate, or QHOL, containing four ply orientations. The lamination parameters for this laminate, i.e. the coordinates (ξ 1, ξ 2 ) = (ξ 9, ξ 10 ) = (0.0, 0.2) on Fig. 4(d), are derived from Eqs. (21): and Eqs. (22): ξ 1 = {n ± cos(2θ ± ) + n cos(2θ ) + n cos(2θ )}/n ξ 1 = {8 cos(90 ) + 6 cos(0 ) + 6 cos(180 )}/20 = 0.0 ξ 2 = {n ± cos(4θ ± ) + n cos(4θ ) + n cos(4θ )}/n ξ 2 = {8 cos(180 ) + 6 cos(0 ) + 6 cos(360 )}/20 = 0.2 ξ 9 = {ζ ± cos(2θ ± ) + ζ cos(2θ ) + ζ cos(2θ )}/ζ ξ 9 = {3200 cos(90 ) cos(0 ) cos(180 )}/8000 = 0.0 ξ 10 = {ζ ± cos(4θ ± ) + ζ cos(4θ ) + ζ cos(4θ )}/ζ ξ 10 = {3200 cos(180 ) cos(0 ) cos(360 )}/8000 =
16 VI. Conclusions This article presents the definitive set of stacking sequences for (82) QuasiHomogeneous Orthotropic Laminates (QHOLs), (973) π/3 and (92) π/4 Extensionally Isotropic Laminates (EILs) and (36) π/3 Fully Isotropic Laminates (FOLs), all of which are subsets from a definitive list of (69,506) stacking sequences for Fully Orthotropic Laminates (FOLs) with up to 21 plies. The great majority of sequences are nonsymmetric in form and many are without any subsequence patterns, e.g. symmetry or repeating groups, which is contrary to the assumptions on which many previous studies have been based. Standard ply angles (±45 /0 /90 for π/4 isotropy and ±60 /0 for π/3 isotropy) have been assumed in the presentation of the feasible domains of lamination parameters commonly adopted in the optimum design of composite laminates, however the stacking sequences are otherwise generic in the sense that any orientation may be assigned to the angleply subsequence, and the two crossply orientations may be arbitrarily switched. For EIL or FIL properties of course, the choice of these arbitrary ply angles must ensure that π/3 or π/4 ply separation is maintained; the stacking sequences otherwise degenerate into FOLs and QHOLs respectively. The ABD relation has been shown to be readily calculated for any general orthotropic fiber/matrix material using the nondimensional stiffness parameters provided. FILs provide an important set of benchmark configurations, which permit like with like comparisons for laminates with other characteristics. References 1 Engineering Sciences Data Unit, Stiffnesses of laminated plates, ESDU Item No , York, C. B., On composite laminates with extensionalanisotropy, Proc. 49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conf., Schaumburg, Illinois, 2008, Accepted for publication. 3 York, C. B., Laminate stacking sequences for special orthotropy, University of Glasgow, Department of Aerospace Engineering Research Report No , York, C. B., Characterization of nonsymmetric forms of fully orthotropic laminates. AIAA Journal of Aircraft, Accepted for publication. See also, York, C. B. Characterization and ply mixing rules for nonsymmetric forms of fully orthotropic laminates, Proc. 48th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conf., AIAA , Honolulu, Hawaii, Wu, K., M. and Avery, B. L., Fully isotropic laminates and quasihomogeneous anisotropic laminates, Journal of Composite Materials, Vol. 26, No. 14, 1992, pp Fukunaga, H., Sekine, H., Sato, M. and Iino, A., Buckling design of symmetrically laminated plates using lamination parameters Computers and Structures, Vol. 57, No. 4, 1995, pp Valot, E. and Vannucci, P., Some exact solutions for fully orthotropic laminates, Composite Structures, Vol. 69, 2005, pp Vannucci, P. and Verchery, G., A new method for generating fully isotropic laminates, Composite Structures, Vol. 58, 2002, pp Caprino, G. and CrivelliVisconti, I., A note on specially orthotropic laminates, Journal of Composite Materials, Vol. 16, No. 5, 1982, Vannucci, P. and Verchery, G., Stiffness design of laminates using the polar method, International Journal of Solids and Structures, Vol. 38, 2001, pp Tsai, S. W. and Pagano, N. J., Composite materials workshop, in: Tsai S. W. et al., editors, Technomic, USA, Bartholomew, P., Ply stacking sequences for laminated plates having inplane and bending orthotropy, Royal Aircraft Establishment Technical Report No , Bartholomew, P., Ply stacking sequences for laminated plates having inplane and bending orthotropy, Fibre Science and Technology, Vol. 10, No. 4, 1977, pp Engineering Sciences Data Unit, Laminate stacking sequences for special orthotropy (Application to fibre reinforced composites), ESDU Item No , Fukunaga, H., and Vanderplaats, G. N., Stiffness optimization of orthotropic laminated composites using lamination parameters, AIAA Journal, Vol. 29, No. 4, 1991, pp Vannucci, P. and Verchery, G., A special class of uncoupled and quasihomogeneous laminates, Composites Science and Technology, Vol. 61, 2001, pp York, C. B., Buckling interaction in regular arrays of rigidly supported composite laminated plates with orthogrid, isogrid and anisogrid planform, AHS Journal, Vol. 52, No. 4, 2007, pp York, C. B., Buckling analysis and minimum mass design procedures for composite wing box structures, AIAA Journal of Aircraft, Vol. 43, No. 2, 2006, pp
17 Appendix Table 7 Fully uncoupled EILs, with π/3 isotropy, for 7 through 21 ply laminates corresponding to prefix designations: (a) AS for Antisymmetric (A) angleplies and Symmetric (S) crossplies; (b) + NN + for Nonsymmetric (N) angleplies and Nonsymmetric (N) crossplies; (c) + NN and; (d) + NN. For all sequences, n ± = 2n, n = n ± + n and ζ = n 3 = ζ ± + ζ. (a) Ref. Sequence n ζ ± ζ AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS Continued 17
18 Continued AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS Continued 18
19 Continued AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS Continued 19
20 Continued AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS AS Concluded 20
21 (b) Ref. Sequence n ζ ± ζ NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN NN Continued 21
A copy can be downloaded for personal noncommercial research or study, without prior permission or charge
York, C. (2015) On tapered warpfree laminates with singleply terminations. Composites Part A: Applied Science and Manufacturing, 72, pp. 127138. Copyright 2015 Elsevier Ltd. A copy can be downloaded
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationCombined Stresses and Mohr s Circle. General Case of Combined Stresses. General Case of Combined Stresses con t. Twodimensional stress condition
Combined Stresses and Mohr s Circle Material in this lecture was taken from chapter 4 of General Case of Combined Stresses Twodimensional stress condition General Case of Combined Stresses con t The normal
More informationIntroduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams.
Outline of Continuous Systems. Introduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams. Vibrations of Flexible Strings. Torsional Vibration of Rods. BernoulliEuler Beams.
More informationQuestion 1. Ignore bottom surface. Solution: Design variables: X = (R, H) Objective function: maximize volume, πr 2 H OR Minimize, f(x) = πr 2 H
Question 1 (Problem 2.3 of rora s Introduction to Optimum Design): Design a beer mug, shown in fig, to hold as much beer as possible. The height and radius of the mug should be not more than 20 cm. The
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationACCURATE FREE VIBRATION ANALYSIS OF POINT SUPPORTED MINDLIN PLATES BY THE SUPERPOSITION METHOD
Journal of Sound and Vibration (1999) 219(2), 265 277 Article No. jsvi.1998.1874, available online at http://www.idealibrary.com.on ACCURATE FREE VIBRATION ANALYSIS OF POINT SUPPORTED MINDLIN PLATES BY
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationUnit 15 Shearing and Torsion (and Bending) of Shell Beams
Unit 15 Shearing and Torsion (and Bending) of Shell Beams Readings: Rivello Ch. 9, section 8.7 (again), section 7.6 T & G 126, 127 Paul A. Lagace, Ph.D. Professor of Aeronautics & Astronautics and Engineering
More informationCORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS
CORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS By Edmond P. Saliklis 1 and Robert H. Falk ABSTRACT: The weakness of existing relationships correlating offaxis modulus of elasticity
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationLinear plate bending and laminate theory
Linear plate bending and laminate theor 4M: Design Tools Eindhoven Universit of Technolog Linear plate bending A plate is a bod of which the material is located in a small region around a surface in the
More informationDr. Michael P. Nemeth
Dr. Michael P. Nemeth Mike Nemeth (2006) From: M. P. Nemeth, Buckling analysis for stiffened anisotropic circular cylinders based on Sanders nonlinear shell theory, NASA/TM2014218176, March 2014 Mike
More informationStress, Strain, Mohr s Circle
Stress, Strain, Mohr s Circle The fundamental quantities in solid mechanics are stresses and strains. In accordance with the continuum mechanics assumption, the molecular structure of materials is neglected
More informationFlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal Unbraced Lengths
Proceedings of the Annual Stability Conference Structural Stability Research Council San Antonio, Texas, March 2124, 2017 FlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal
More informationAnalysis and Optimization of a Hybrid Fan Blade
Analysis and Optimization of a Hybrid Fan Blade Permas Users Conference 27.04.06 28.04.06 Strassbourg DLR German Aerospace Center, Stuttgart Institute of Structures and Design J. Ehrmanntraut, F. Kocian,
More information*MAT_PAPER  a new orthotropic elastoplastic model for paper materials
*MAT_PAPER  a new orthotropic elastoplastic model for paper materials Jesper Karlsson, Dynamore Nordic Mikael Schill, Dynamore Nordic Johan Tryding, Tetra Pak *MAT_PAPER (*MAT_274) A new orthotropic elastoplastic
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationMohr's Circle for 2D Stress Analysis
Mohr's Circle for 2D Stress Analysis If you want to know the principal stresses and maximum shear stresses, you can simply make it through 2D or 3D Mohr's cirlcles! You can know about the theory of
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationMATRIX ALGEBRA AND SYSTEMS OF EQUATIONS. + + x 1 x 2. x n 8 (4) 3 4 2
MATRIX ALGEBRA AND SYSTEMS OF EQUATIONS SYSTEMS OF EQUATIONS AND MATRICES Representation of a linear system The general system of m equations in n unknowns can be written a x + a 2 x 2 + + a n x n b a
More informationUniversity of Bristol  Explore Bristol Research. Publisher's PDF, also known as Version of record License (if available): Unspecified
Garza Rodriguez, C., Smith, D., Shterenlikht, A., & Pavier, M. (2015). Advances in the deep hole drilling technique for the residual stress measurement in composite laminates. In Proc 5th Thematic Conf.
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationFinite Math  Jterm Section Systems of Linear Equations in Two Variables Example 1. Solve the system
Finite Math  Jterm 07 Lecture Notes  //07 Homework Section 4.  9, 0, 5, 6, 9, 0,, 4, 6, 0, 50, 5, 54, 55, 56, 6, 65 Section 4.  Systems of Linear Equations in Two Variables Example. Solve the system
More informationModeling of FiberReinforced Membrane Materials Daniel Balzani. (Acknowledgement: Anna Zahn) Tasks Week 2 Winter term 2014
Institute of echanics and Shell Structures Faculty Civil Engineering Chair of echanics odeling of FiberReinforced embrane aterials OOC@TU9 Daniel Balani (Acknowledgement: Anna Zahn Tasks Week 2 Winter
More informationAnd similarly in the other directions, so the overall result is expressed compactly as,
SQEP Tutorial Session 5: T7S0 Relates to Knowledge & Skills.5,.8 Last Update: //3 Force on an element of area; Definition of principal stresses and strains; Definition of Tresca and Mises equivalent stresses;
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationGLOBAL AND LOCAL LINEAR BUCKLING BEHAVIOR OF A CHIRAL CELLULAR STRUCTURE
GLOBAL AND LOCAL LINEAR BUCKLING BEHAVIOR OF A CHIRAL CELLULAR STRUCTURE Alessandro Spadoni, Massimo Ruzzene School of Aerospace Engineering Georgia Institute of Technology Atlanta, GA 30332 Fabrizio Scarpa
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More information7. STRESS ANALYSIS AND STRESS PATHS
71 7. STRESS ANALYSIS AND STRESS PATHS 7.1 THE MOHR CIRCLE The discussions in Chapters and 5 were largely concerned with vertical stresses. A more detailed examination of soil behaviour requires a knowledge
More informationA review on the mechanical behaviour of curvilinear fibre composite laminated panels
A review on the mechanical behaviour of curvilinear fibre composite laminated panels Pedro Ribeiro, Hamed Ahavan IDMEC/DEMec, Faculdade de Engenharia, Universidade do Porto Porto, Portugal Andrzej Teter,
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationNonlinear Analysis of Reinforced Concrete Shells Subjected to Impact Loads
Transactions of the 7 th International Conference on Structural Mechanics in Reactor Technology (SMiRT 7) Prague, Czech Republic, August 7, 00 Paper # J0 Nonlinear Analysis of Reinforced Concrete Shells
More informationBy drawing Mohr s circle, the stress transformation in 2D can be done graphically. + σ x σ y. cos 2θ + τ xy sin 2θ, (1) sin 2θ + τ xy cos 2θ.
Mohr s Circle By drawing Mohr s circle, the stress transformation in D can be done graphically. σ = σ x + σ y τ = σ x σ y + σ x σ y cos θ + τ xy sin θ, 1 sin θ + τ xy cos θ. Note that the angle of rotation,
More informationEffects of a pulsed electromagnetic field on the impact response of electrically conductive. composite plates
Effects of a pulsed electromagnetic field on the impact response of electrically conductive composite plates 1. Introduction Electromagnetic solids encompass a broad class of materials in which the interaction
More informationAnalysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements
Acta Mech. Sin. (2016) 32(2):295 300 DOI 10.1007/s1040901505342 RESEARCH PAPER Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements V. H. Carneiro 1
More informationCOURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.)
Narvik University College (Høgskolen i Narvik) EXAMINATION TASK COURSE STE6289 Modern Materials and Computations (Moderne materialer og beregninger 7.5 stp.) CLASS: Master students in Engineering Design
More informationFEM Modeling of a 3D Printed Carbon Fiber Pylon
FEM Modeling of a 3D Printed Carbon Fiber Pylon I. López G.*, B. Chiné, and J.L. León S. Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding
More informationMechanics of Materials MENG 270 Fall 2003 Exam 3 Time allowed: 90min. Q.1(a) Q.1 (b) Q.2 Q.3 Q.4 Total
Mechanics of Materials MENG 70 Fall 00 Eam Time allowed: 90min Name. Computer No. Q.(a) Q. (b) Q. Q. Q.4 Total Problem No. (a) [5Points] An air vessel is 500 mm average diameter and 0 mm thickness, the
More informationResearch Article Behaviour and Optimization Aids of Composite Stiffened Hypar Shell Roofs with Cutout under Free Vibration
International Scholarly Research Network ISRN Civil Engineering Volume 2012, Article ID 989785, 14 pages doi:10.5402/2012/989785 Research Article Behaviour and Optimization Aids of Composite Stiffened
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationWrinkling Analysis of A Kapton Square Membrane under Tensile Loading
44th AIAA/ASME/ASCE/AHS Structures, Structural Dynamics, and Materials Confere 710 April 2003, Norfolk, Virginia AIAA 20031985 Wrinkling Analysis of A Kapton Square Membrane under Tensile Loading Xiaofeng
More informationChapter 3 LAMINATED MODEL DERIVATION
17 Chapter 3 LAMINATED MODEL DERIVATION 3.1 Fundamental Poisson Equation The simplest version of the frictionless laminated model was originally introduced in 1961 by Salamon, and more recently explored
More informationUSE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR
USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationSection Downloads. Section Downloads. Handouts & Slides can be printed. Other documents cannot be printed Course binders are available for purchase
Level II: Section 04 Simplified Method (optional) Section Downloads Section Downloads Handouts & Slides can be printed Version.0 Other documents cannot be printed Course binders are available for purchase
More informationTHE BENDING STIFFNESSES OF CORRUGATED BOARD
AMDVol. 145/MDVol. 36, Mechanics of Cellulosic Materials ASME 1992 THE BENDING STIFFNESSES OF CORRUGATED BOARD S. Luo and J. C. Suhling Department of Mechanical Engineering Auburn University Auburn,
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationTHE MECHANICAL BEHAVIOR OF ORIENTED 3D FIBER STRUCTURES
Lappeenranta University of Technology School of Engineering Science Degree Program in Computational Engineering and Technical Physics Master s Thesis Alla Kliuzheva THE MECHANICAL BEHAVIOR OF ORIENTED
More informationDesign of reinforced concrete sections according to EN and EN
Design of reinforced concrete sections according to EN 199211 and EN 19922 Validation Examples Brno, 21.10.2010 IDEA RS s.r.o. South Moravian Innovation Centre, U Vodarny 2a, 616 00 BRNO tel.: +420511
More information1 Introduction. Keywords: stiffened hypar shell; cutout; antisymmetric angle ply composite; finite element method
Curved and Layer. Struct. 2016; (3) 1:22 46 Research Article Open Access Puja B. Chowdhury, Anirban Mitra, and Sarmila Sahoo* Relative performance of antisymmetric angleply laminated stiffened hypar shell
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationPLATE GIRDERS II. Load. Web plate Welds A Longitudinal elevation. Fig. 1 A typical Plate Girder
16 PLATE GIRDERS II 1.0 INTRODUCTION This chapter describes the current practice for the design of plate girders adopting meaningful simplifications of the equations derived in the chapter on Plate Girders
More informationLocalization in Undrained Deformation
Localization in Undrained Deformation J. W. Rudnicki Dept. of Civil and Env. Engn. and Dept. of Mech. Engn. Northwestern University Evanston, IL 621319 John.Rudnicki@gmail.com Fourth Biot Conference on
More information(x 1, y 1 ) = (x 2, y 2 ) if and only if x 1 = x 2 and y 1 = y 2.
1. Complex numbers A complex number z is defined as an ordered pair z = (x, y), where x and y are a pair of real numbers. In usual notation, we write z = x + iy, where i is a symbol. The operations of
More informationEmpirical Prediction of Shear Modulus and Young's Modulus of Plywood Panels
Empirical Prediction of Shear Modulus and Young's Modulus of Plywood Panels By Edmond P. Saliklis Assistant Professor of Civil and Environmental Engineering 3 Alumni Hall of Engineering Lafayette College,
More informationProperties of a chiral honeycomb with a Poisson's ratio 1
Properties of a chiral honeycomb with a Poisson's ratio 1 D. Prall, R. S. Lakes Int. J. of Mechanical Sciences, 39, 305314, (1996). Abstract A theoretical and experimental investigation is conducted
More informationModeling of the Bending Stiffness of a Bimaterial Beam by the Approximation of OneDimensional of Laminated Theory
. FloresDomínguez Int. Journal of Engineering Research and Applications RESEARCH ARTICLE OPEN ACCESS odeling of the Bending Stiffness of a Bimaterial Beam by the Approimation of OneDimensional of Laminated
More informationLab Exercise #3: Torsion
Lab Exercise #3: Prelab assignment: Yes No Goals: 1. To evaluate the equations of angular displacement, shear stress, and shear strain for a shaft undergoing torsional stress. Principles: testing of round
More informationL e c t u r e. D r. S a s s a n M o h a s s e b
The Scaled smteam@gmx.ch Boundary Finite www.erdbebenschutz.ch Element Method Lecture A L e c t u r e A1 D r. S a s s a n M o h a s s e b V i s i t i n g P r o f e s s o r M. I. T. C a m b r i d g e December
More informationJournal of Composite Materials. Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios
Behaviour of hollow pultruded GFRP square beams with different shear spantodepth ratios Journal: Manuscript ID: Draft Manuscript Type: Original Manuscript Date Submitted by the Author: n/a Complete List
More informationMECH 344/X Machine Element Design
1 MECH 344/X Machine Element Design Time: M 14:4517:30 Lecture 2 Contents of today's lecture Introduction to Static Stresses Axial, Shear and Torsional Loading Bending in Straight and Curved Beams Transverse
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationAspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites
Aspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a
More informationMulti physics design and optimization of flexible matrix composite (FMC) driveshafts
Research Collection Master Thesis Multi physics design and optimization of flexible matrix composite (FMC) driveshafts Author(s): Roos, Christoph Publication Date: 2010 Permanent Link: https://doi.org/10.3929/ethza010076645
More informationtorsion equations for lateral BucKling ns trahair research report r964 July 2016 issn school of civil engineering
TORSION EQUATIONS FOR ATERA BUCKING NS TRAHAIR RESEARCH REPORT R96 Jul 6 ISSN 878 SCHOO OF CIVI ENGINEERING SCHOO OF CIVI ENGINEERING TORSION EQUATIONS FOR ATERA BUCKING RESEARCH REPORT R96 NS TRAHAIR
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationPLAXIS. Scientific Manual
PLAXIS Scientific Manual 2016 Build 8122 TABLE OF CONTENTS TABLE OF CONTENTS 1 Introduction 5 2 Deformation theory 7 2.1 Basic equations of continuum deformation 7 2.2 Finite element discretisation 8 2.3
More informationDruckerPrager yield criterion application to study the behavior of CFRP confined concrete under compression
XXXVII IAHS World ongress on Housing October 6 9, 00, Santander, Spain DruckerPrager yield criterion application to study the behavior of FRP confined concrete under compression Salvador Ivorra, Ramón
More informationProblem Set 2 Due Tuesday, September 27, ; p : 0. (b) Construct a representation using five d orbitals that sit on the origin as a basis: 1
Problem Set 2 Due Tuesday, September 27, 211 Problems from Carter: Chapter 2: 2ad,g,h,j 2.6, 2.9; Chapter 3: 1ad,f,g 3.3, 3.6, 3.7 Additional problems: (1) Consider the D 4 point group and use a coordinate
More informationFINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND
FINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND COMPARISON WITH EXPERIMENTAL IMPACT TESTS USING NONDESTRUCTIVE VIBROTHERMOGRAPHY EVALUATION A
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationCivil Engineering Design (1) Design of Reinforced Concrete Columns 2006/7
Civil Engineering Design (1) Design of Reinforced Concrete Columns 2006/7 Dr. Colin Caprani, Chartered Engineer 1 Contents 1. Introduction... 3 1.1 Background... 3 1.2 Failure Modes... 5 1.3 Design Aspects...
More informationAdvantages, Limitations and Error Estimation of Mixed Solid Axisymmetric Modeling
Advantages, Limitations and Error Estimation of Mixed Solid Axisymmetric Modeling Sudeep Bosu TATA Consultancy Services Baskaran Sundaram TATA Consultancy Services, 185 Lloyds Road,Chennai600086,INDIA
More informationWEEK 10 Soil Behaviour at Medium Strains
WEEK 10 Soil Behaviour at Medium Strains 14. Onset of yielding 141. What is yielding: Remember? We have already studied what yielding means; if you don t remember, refer back to Week 2. It is defined
More informationARC 341 Structural Analysis II. Lecture 10: MM1.3 MM1.13
ARC241 Structural Analysis I Lecture 10: MM1.3 MM1.13 MM1.4) Analysis and Design MM1.5) Axial Loading; Normal Stress MM1.6) Shearing Stress MM1.7) Bearing Stress in Connections MM1.9) Method of Problem
More information2008 by authors and 2008 Springer Science+Business Media
Antti H. Niemi, Harri Hakula, and Juhani Pitkäranta. 28. Point load on a shell. In: Karl Kunisch, Günther Of, and Olaf Steinbach (editors). Numerical Mathematics and Advanced Applications. Proceedings
More informationAvailable online at ScienceDirect. Procedia Engineering 88 (2014 )
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 88 (2014 ) 242 254 International Symposium on Dynamic Response and Failure of Composite Materials, DRaF2014 Residual strength
More informationPrimary Mirror Cell Deformation and Its Effect on Mirror Figure Assuming a Sixzone Axial Defining System
Primary Mirror Cell Deformation and Its Effect on Mirror Figure Larry Stepp Eugene Huang Eric Hansen Optics Manager Optostructural Engineer Optomechanical Engineer November 1993 GEMINI PROJECT OFFICE
More informationSpherical Pressure Vessels
Spherical Pressure Vessels Pressure vessels are closed structures containing liquids or gases under essure. Examples include tanks, pipes, essurized cabins, etc. Shell structures : When essure vessels
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More informationKirchhoff Plates: Field Equations
20 Kirchhoff Plates: Field Equations AFEM Ch 20 Slide 1 Plate Structures A plate is a three dimensional bod characterized b Thinness: one of the plate dimensions, the thickness, is much smaller than the
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More informationBridge deck modelling and design process for bridges
EURussia Regulatory Dialogue Construction Sector Subgroup 1 Bridge deck modelling and design process for bridges Application to a composite twingirder bridge according to Eurocode 4 Laurence Davaine
More informationEffect of Relative Humidity on the Optimum Flute Shape for Corrugated Fiberboard
Effect of Relative Humidity on the Optimum Flute Shape for Corrugated Fiberboard Thomas J. Urbanik Research Engineer U.S. Department of Agriculture Forest Service Forest Products Laboratory Madison, Wisconsin
More informationTHE USE OF DYNAMIC RELAXATION TO SOLVE THE DIFFERENTIAL EQUATION DESCRIBING THE SHAPE OF THE TALLEST POSSIBLE BUILDING
VII International Conference on Textile Composites and Inflatable Structures STRUCTURAL MEMBRANES 2015 E. Oñate, K.U.Bletzinger and B. Kröplin (Eds) THE USE OF DYNAMIC RELAXATION TO SOLVE THE DIFFERENTIAL
More informationarxiv:quantph/ v1 29 Mar 2003
FiniteDimensional PT Symmetric Hamiltonians arxiv:quantph/0303174v1 29 Mar 2003 Carl M. Bender, Peter N. Meisinger, and Qinghai Wang Department of Physics, Washington University, St. Louis, MO 63130,
More informationWESTERGAARD COMPLEX STRESS FUNCTIONS (16)
GG711c 1/1/03 1 WESTERGAARD COMPLEX STRESS FUNCTIONS (16) I Main topics A B Historical perspective Expression of the biharmonic function by harmonic functions C Boundary conditions D Use of symmetry and
More information